balancing hydrogen adsorption/desorption by orbital ... article balancing hydrogen...
Post on 12-Aug-2020
Embed Size (px)
Balancing hydrogen adsorption/desorption by orbital modulation for efficient hydrogen evolution catalysis Feng Li 1, Gao-Feng Han 1, Hyuk-Jun Noh1, Jong-Pil Jeon1, Ishfaq Ahmad1, Shanshan Chen2,3,
Changduk Yang 3, Yunfei Bu4, Zhengping Fu5, Yalin Lu 5 & Jong-Beom Baek 1
Hydrogen adsorption/desorption behavior plays a key role in hydrogen evolution reaction
(HER) catalysis. The HER reaction rate is a trade-off between hydrogen adsorption and
desorption on the catalyst surface. Herein, we report the rational balancing of hydrogen
adsorption/desorption by orbital modulation using introduced environmental electronegative
carbon/nitrogen (C/N) atoms. Theoretical calculations reveal that the empty d orbitals of
iridium (Ir) sites can be reduced by interactions between the environmental electronegative
C/N and Ir atoms. This balances the hydrogen adsorption/desorption around the Ir sites,
accelerating the related HER process. Remarkably, by anchoring a small amount of Ir
nanoparticles (7.16 wt%) in nitrogenated carbon matrixes, the resulting catalyst exhibits
significantly enhanced HER performance. This includs the smallest reported overpotential at
10mA cm−2 (4.5 mV), the highest mass activity at 10 mV (1.12 A mgIr−1) and turnover fre-
quency at 25mV (4.21 H2 s−1) by far, outperforming Ir nanoparticles and commercial Pt/C.
1 School of Energy and Chemical Engineering/Center for Dimension-Controllable Organic Frameworks, Ulsan National Institute of Science and Technology (UNIST), 50 UNIST, Ulsan 44919, South Korea. 2MOE Key Laboratory of Low-grade Energy Utilization Technologies and Systems, CQU-NUS Renewable Energy Materials & Devices Joint Laboratory, School of Energy & Power Engineering, Chongqing University, Chongqing 400044, P. R. China. 3 Department of Energy Engineering, School of Energy and Chemical Engineering, Perovtronics Research Center, Low Dimensional Carbon Materials Center, Ulsan National Institute of Science and Technology (UNIST), 50 UNIST, Ulsan 44919, South Korea. 4 School of Environmental Science and Engineering, Nanjing University of Information Science and Technology, 219 Ningliu, Nanjing, Jiangsu 210044, P. R. China. 5 CAS Key Laboratory of Materials for Energy Conversion, Hefei National Laboratory for Physical Sciences at Microscale, National Synchrotron Radiation Laboratory, University of Science and Technology of China, 96 Jinzhai, Hefei, Anhui 230026, P. R. China. Correspondence and requests for materials should be addressed to Y.B. (email: email@example.com) or to Z.F. (email: firstname.lastname@example.org) or to J.-B.B. (email: email@example.com)
NATURE COMMUNICATIONS | (2019) 10:4060 | https://doi.org/10.1038/s41467-019-12012-z | www.nature.com/naturecommunications 1
9 0 () :,;
http://orcid.org/0000-0002-9891-8260 http://orcid.org/0000-0002-9891-8260 http://orcid.org/0000-0002-9891-8260 http://orcid.org/0000-0002-9891-8260 http://orcid.org/0000-0002-9891-8260 http://orcid.org/0000-0001-5943-0492 http://orcid.org/0000-0001-5943-0492 http://orcid.org/0000-0001-5943-0492 http://orcid.org/0000-0001-5943-0492 http://orcid.org/0000-0001-5943-0492 http://orcid.org/0000-0001-7452-4681 http://orcid.org/0000-0001-7452-4681 http://orcid.org/0000-0001-7452-4681 http://orcid.org/0000-0001-7452-4681 http://orcid.org/0000-0001-7452-4681 http://orcid.org/0000-0001-8240-5404 http://orcid.org/0000-0001-8240-5404 http://orcid.org/0000-0001-8240-5404 http://orcid.org/0000-0001-8240-5404 http://orcid.org/0000-0001-8240-5404 http://orcid.org/0000-0003-4785-2326 http://orcid.org/0000-0003-4785-2326 http://orcid.org/0000-0003-4785-2326 http://orcid.org/0000-0003-4785-2326 http://orcid.org/0000-0003-4785-2326 mailto:firstname.lastname@example.org mailto:email@example.com mailto:firstname.lastname@example.org www.nature.com/naturecommunications www.nature.com/naturecommunications
Because of its potential value in efficient and scalablehydrogen production, water splitting via the electro-chemical hydrogen evolution reaction (HER) has attracted considerable attention from industrial and scientific communities1,2. Even though they are the heart of hydrogen evolution catalysis, catalysts with satisfactory performance are still rare, despite the tremendous effort that has been devoted to improving HER catalysts3–11. Among various approaches, sulfur (S) vacancies and strain have been introduced to activate and optimize the basal plane of monolayer 2H–MoS2, leading to the highest intrinsic HER activity among molybdenum–sulfide-based catalysts8. A high concentration of strained metallic 1T WS2 sites, obtained by chemical exfoliation, led to WS2 nanosheets with enhanced catalytic activity4. Ultrathin Pt nanowires on single- layered Ni(OH)2 nanosheets with a unique hybrid nanostructure were also achieved, and exhibited unprecedented catalytic activity and stability toward HER6. Nonetheless, in spite of these achievements, strategic exploration to improve the HER perfor- mance of catalysts is still a great challenge.
From a fundamental viewpoint, the hydrogen adsorption/des- orption behaviors of the solid surfaces of catalysts are of crucial importance in hydrogen evolution catalysis12,13. Stronger hydrogen adsorption enables faster proton supply for the reac- tion, however, on the other side, this leads to weaker hydrogen desorption and slower release of active sites. Too strong or too weak hydrogen adsorption/desorption will lead to either active site poisoning or inefficient proton supply, resulting in a sluggish hydrogen evolution reaction rate.
The hydrogen adsorption/desorption behaviors of transition metal-based catalysts depend largely on the interaction between the unfulfilled d orbitals of the transition metals and the s orbital of hydrogen14. As a result, hydrogen adsorption/deso- rption on such catalysts can be tailored by tuning the d orbitals of the transition metals. With their small atomic radius and high electronegativity, the p orbitals of carbon and nitrogen are able to efficiently interact with the d orbitals of the transition metals15. This provides an important opportunity to enhance the catalytic activity of catalysts toward HER via orbital manipulation.
Herein, we demonstrate the rational balancing of hydrogen adsorption/desorption on a solid catalyst surface to archive significantly enhanced hydrogen evolution performance via orbital modulation. Density functional theory (DFT) calcula- tions revealed that the empty d orbitals of iridium (Ir) sites can be tailored by an electronegative carbon/nitrogen (C/N) environment, which will further balance hydrogen adsorption/ desorption behaviors and boost the hydrogen evolution cata- lysis on the surficial Ir sites. Importantly, even with a low-Ir concentration of 7.16 wt%, when Ir nanoparticles (IrNP) were anchored on a hollow nitrogenated carbon matrix (IrHNC), the resulting catalyst exhibited HER performance superior to IrNP and commercial Pt/C, including much faster reaction kinetics, and much higher mass activity as well as intrinsic activity.
Results DFT calculations. Figure 1 shows the different hydrogen adsorption/desorption behaviors on the solid surface of catalyst. For an efficient HER, fast reactant supply and fast product delivery are needing to be satisfied simultaneously, which required strong hydrogen adsorption and strong hydrogen des- orption capabilities from the catalyst surface. However, as the two sides of the coin, they cannot be achieved at the same time. Thus, the hydrogen adsorption/desorption behaviors balancing offers an alternative way to enhance the HER performance of the catalysts.
With a weak hydrogen adsorption behavior, Ir was first selected for the hydrogen adsorption/ desorption behavior balancing16. As the thermally stable plane of Ir, the (111) plane is most stable and available in the experiment. Thus, the theoretical investigations were conducted on its thermally stable (111) plane. The structures of the calculation models for Ir without/with C/N environment (Ir/IrNC) are shown in Supple- mentary Figs. 1 and 2. The orbital profiles of Ir and IrNC were analyzed first. Figure 2 shows the different views of the orbitals above the Fermi level for Ir and IrNC, which are predominately composed of empty d orbitals for Ir sites. The empty d orbitals above the Fermi level in Fig. 2a, b, along with the projected density of states (DOS) distributions of the Ir, C, and N sites (Supplementary Fig. 3), reveal the strong interactions between the Ir and environmental C/N sites. Because of a large wave function overlap, the p orbitals of the C/N sites directly interact with the dz2 orbitals of the nearby Ir sites. By introducing the C/N environment, the empty d orbitals of the surficial Ir sites for IrNC were remarkably reduced, benefiting the activation of surficial Ir sites and electron transport on the Ir surface of IrNC (Fig. 2c, d).
The orbital modulated electron structure of IrNC can be further illustrated using the electron density difference calcula- tion, with Ir as the reference (Supplementary Fig. 4). The electrons of the surficial Ir sites on the Ir(111) surface are more like to transfer to nearby hollow fcc sites. Thus, the hollow fcc sites with high electron density are favored for hydrogen adsorption. Compared with Ir, the electron density of the surficial Ir sites of IrNC is much lower, while it is exactly the opposite for the hollow fcc sites. Therefore, the hollow fcc sites on the surface of IrNC with higher electron density will benefit hydrogen adsorption, leading to enhanced HER performance. Furthermore, the positive shift of the d-band center toward the Fermi level (EF) in IrNC agrees well with